O R I G I N A L PA P E R
Muon-Spin Rotation and Magnetization Studies of Chemical
and Hydrostatic Pressure Effects in EuFe
Z. Guguchia· A. Shengelaya · A. Maisuradze ·
L. Howald· Z. Bukowski · M. Chikovani · H. Luetkens · S. Katrych· J. Karpinski · H. Keller
Received: 24 July 2012 / Accepted: 30 July 2012 / Published online: 25 August 2012 © Springer Science+Business Media, LLC 2012
Abstract The magnetic phase diagram of EuFe2(As1−xPx)2 was investigated by means of magnetization and muon-spin rotation (μSR) studies as a function of chemical (isovalent substitution of As by P) and hydrostatic pressure. The mag-netic phase diagrams of the magmag-netic ordering of the Eu and Fe spins with respect to P content and hydrostatic pressure are determined and discussed. The present investigations re-veal that the magnetic coupling between the Eu and the Fe sublattices strongly depends on chemical and hydrostatic
Z. Guguchia ()· A. Maisuradze · L. Howald · H. Keller Physik-Institut der Universität Zürich, Winterthurerstrasse 190, 8057 Zürich, Switzerland
A. Shengelaya· M. Chikovani
Department of Physics, Tbilisi State University, Chavchavadze 3, 0128 Tbilisi, Georgia
Laboratory for Developments and Methods, Paul Scherrer Institute, 5232 Villigen PSI, Switzerland
A. Maisuradze· H. Luetkens
Laboratory for Muon Spin Spectroscopy, Paul Scherrer Institute, 5232 Villigen PSI, Switzerland
Institute of Low Temperature and Structure Research, Polish Academy of Sciences, 50-422 Wroclaw, Poland
Z. Bukowski· S. Katrych · J. Karpinski
Laboratory for Solid State Physics, ETH Zürich, 8093 Zürich, Switzerland
S. Katrych· J. Karpinski
Institut de Physique de la Matiére Condensée (ICMP), Ecole Polytechnique Fédérale de Lausanne (EPFL), 1015 Lausanne, Switzerland
pressure. It is found that chemical and hydrostatic pressures have a similar effect on the Eu and Fe magnetic order.
Keywords High temperature Fe-based superconductor· Localized and band magnetism· Hydrostatic pressure · Chemical pressure
The discovery of superconductivity in the iron-based pnic-tides  provided a new class of compounds to the high temperature superconductor (HTS) family. Ternary iron ar-senide AFe2As2(A= Sr, Ca, Ba, Eu)  is one of the par-ent compounds with ThCr2Si2-type structure. Similarly as LnFeAsO (Ln= La–Gd) , AFe2As2undergoes a struc-tural phase transition from a tetragonal to an orthorom-bic phase, accompanied or followed by a spin-density-wave (SDW) transition of the itinerant Fe moments. The super-conducting (SC) state can be achieved either under pressure (chemical and hydrostatic) [4–6] or by appropriate charge carrier doping of the parent compounds [7–9], both accom-panied by a suppression of the SDW state.
Here, we focus on EuFe2As2which is a particularly inter-esting member of the ternary system AFe2As2, since the A site is occupied by a rare earth Eu2+S-state (orbital moment L= 0) ion with a 4f7electronic configuration. Eu2+has a total electron spin S= 7/2, corresponding to a theoretical effective magnetic moment of μeff= 7.94 μB. In addition to the SDW ordering of the Fe moments at TSDW 190 K, an antiferromagnetic (AFM) order of the Eu2+spins at TAFM 19 K was reported by Mössbauer spectroscopy  and later confirmed by neutron diffraction . Various reports on EuFe2−xCoxAs2(x= 0 and 0.1) suggest a strong coupling between the magnetism of the Eu2+ions and the conduction electrons, which may affect or even destroy
superconductiv-ity [12,13]. For example, in contrast to the other ‘122’ sys-tems, where the substitution of Fe by Co leads to supercon-ductivity [14,15], the compounds containing Eu2+ exhibit the onset of a superconducting transition, but seem to be hindered to reach zero resistivity at ambient pressure . Although Ni doping in BaFe2As2leads to superconductivity up to 21 K , ferromagnetism rather than superconductiv-ity was found in EuFe2As2by Ni doping . On the other hand, in single crystals of P substituted EuFe2(As1−xPx)2 bulk superconductivity with superconducting transition tem-perature Tc 28 K was observed by resistivity, magnetiza-tion, and specific heat measurements . Isovalent P sub-stitution on the As site in EuFe2As2 without introducing holes or electrons simulates a condition generally referred to as “chemical pressure”. Superconductivity coexisting with AFM Eu2+order was only found in a very narrow range of P content x (0.16≤ x ≤ 0.22), where the SDW transition is suppressed. Superconductivity with a zero resistivity state was also observed for EuFe2As2 under applied pressure [6,20]. Similar to the case of P substitution, superconduc-tivity covers only a narrow pressure range of 2.5–3.0 GPa.
In this paper, we report detailed magnetization and muon spin rotation (μSR) measurements in EuFe2As2−xPx as a function of the P content x. One P substituted sample EuFe2(As0.88P0.12)2 was also studied under applied pres-sure p. The μSR technique is a powerful tool to study the magnetic and superconducting properties of materials microscopically. It provides reliable measurements of Tc, TSDW, the magnetic ordering temperature of Eu2+ spins TEu and the ordered moment size as a function of both x and p. Consequently, the phase diagrams with respect x and pare determined from these measurements. We compare the present results with previous high pressure studies on the parent compound EuFe2As2 and discuss the combined re-sults in terms of the relation of x and p. The paper is or-ganized as follows: Experimental details are described in Sect. 2. The results of the magnetic susceptibility and the μSR experiments at ambient and applied pressure are pre-sented and discussed in Sects.3.1and3.2, respectively. In Sect.4, the phase diagrams are presented. The conclusions follow in Sect.5.
2 Experimental Details
In the present work, the system EuFe2(As1−xPx)2 with x = 0, 0.12, 0.2, and 1 is investigated. Note that the sam-ple with x= 0 is single crystalline, and all the P substi-tuted compounds are pollycrystalline. The concentrations x= 0.12 and 0.2 were studied due to their proximity to the SC phase reported in . A single crystal of EuFe2As2was grown out of Sn flux . Polycrystalline samples were syn-thesized by solid-state reaction between EuAs, Fe2As, and Fe2P. EuAs was presynthesized by heating europium grains and phosphorus powders very slowly to 1173 K followed
by a tempering at this temperature for 36 h. Fe2As was pre-pared by heating Fe and As powders at 973 K for 10 h and at 1173 K for 15 h. Fe2P was presynthesized by reacting iron and phosphorus powders at 973 K for 24 h from sto-ichiometric amounts of the elements. All the starting ma-terials had a purity better than 99.9 %. Powders of EuAs, Fe2As, and Fe2P were weighted according to the stoichio-metric ratio, thoroughly ground and pressed into pellets in an argon-filled glove box. The pellets were then sealed in an evacuated quartz tube, sintered at 1273 K for 36 h, and then cooled slowly to room temperature.
Powder X-ray diffraction (XRD) studies of the EuFe2(As1−xPx)2 samples were carried out at room tem-perature with a STOE diffractometer (CuKα1 radiation, λ= 1.5406 Å) equipped with a mini-phase-sensitive de-tector and a Ge monochromator. The structural refinements were done using the program FULLPROF . The zero-field-cooled and zero-field-cooled (ZFC and FC) magnetization measurements of the EuFe2(As1−xPx)2 samples were per-formed with a commercial SQUID magnetometer (Quantum Design MPMS-XL). The samples with x= 0.2 and 1 were studied only at ambient pressure. For x= 0.12, the investi-gations were also carried out under applied pressures up to p= 5.9 GPa by using a diamond anvil cell (DAC) filled with Daphne oil which served as a pressure-transmitting medium. The pressure at low temperatures was determined by the pressure dependence of the SC transition temperature of Pb. Zero-field (ZF) μSR experiments were performed at the μE1 and π M3 beamlines of the Paul Scherrer Insti-tute (Villigen, Switzerland). The general purpose instru-ment (GPS) was used to study the system EuFe2(As1−xPx)2 (x= 0, 0.12, 0.2, and 1) at ambient pressure. The sam-ples were mounted inside of a gas-flow 4He cryostat on a sample holder with a standard veto setup providing a low-background μSR signal. In addition, the sample with x= 0.12 was studied under pressure using the GPD instru-ment. Pressures up to 2.0 GPa were generated in a double wall piston-cylinder type of cell made of MP35N  ma-terial especially designed to perform μSR experiments un-der pressure. As a pressure transmitting medium Daphne oil was used. The pressure was measured by tracking the SC transition of a very small indium plate by AC susceptibility. The μSR time spectra were analyzed using the free software package MUSRFIT .
3 Results and Discussion
3.1 Crystal Structure and Magnetic Properties of EuFe2(As1−xPx)2
3.1.1 X-Ray Powder Diffraction
The crystal structure for all EuFe2(As1−xPx)2 samples at room temperature was refined with the tetragonal ThCr2Si2
Fig. 1 X-ray powder diffraction pattern at room temperature for the
sample EuFe2(As0.88P0.12)2. The solid line represents a Ritveld
refine-ment profile. The residuals are plotted at the bottom of the figure. In the
inset, refined lattice parameters are plotted as a function of P content x
structure. An example of the refinement profile for EuFe2(As0.88P0.12)2 is shown in Fig. 1. No obvious sec-ondary phase can be detected. The weighted pattern fac-tor and goodness of fit are Rwp∼ 11.2 % and S ∼ 1.6, respectively, indicating a fairly good refinement. In ad-dition, the refined occupancies are close to the nominal values. The lattice constants for the tetragonal unit cell based upon the Rietveld refinements are a= 3.9095(2) Å and c = 11.979(1) Å for x = 0.12, a = 3.9006(2) Å and c= 11.9312(1) Å for x = 0.2, a = 3.8152(2) Å and c= 11.2401(1) Å for x = 1. The values for x = 1 are in agreement with the literature values [a= 3.8178(1) Å and c= 11.2372(3) Å] . The lattice constants a and c as a function of x are plotted in the inset of Fig. 1. A de-crease of both a and c with increasing x is observed. The decrease of the lattice constant c as a result of P substi-tution implies an increase of the coupling between the Eu and the Fe2(As1−xPx)2layers. This might also be important for the evolution of the magnetic order in the Eu-sublattice, since the Ruderman–Kittel–Kasuya–Yosida (RKKY) cou-pling strongly depends on the distance between the magnetic ions [13,18,25].
3.1.2 Magnetization Measurements
The temperature dependence of the zero-field-cooled (ZFC) and field-cooled (FC) magnetic susceptibility χ= M/H for EuFe2(As1−xPx)2(x= 0.12, 0.2, and 1) in a magnetic field of μ0H= 2 mT is shown in Fig. 2. The results for x= 0 were already discussed in detail in our previous work , and hence, are not shown here. The magnetic susceptibility at high temperatures (i.e., far above the magnetic ordering temperature of the Eu2+moments T
Eu) is well described by
Fig. 2 Temperature dependence of the ZFC and FC magnetic
suscep-tibility for the samples EuFe2(As1−xPx)2(x= 0.12, 0.2, 1) measured
in a magnetic field of μ0H= 2 mT. The inset illustrates the
tempera-ture dependence of the difference of both susceptibilities (χFC−χZFC).
The arrows mark the magnetic ordering temperatures TEuof the Eu2+
the Curie–Weiss law: χ (T )= C
T − θCW
Here, C denotes the Curie constant and θCW the paramag-netic Curie–Weiss temperature. An analysis of the data in Fig.2with Eq. (1) yields: θCW= 16.74(8) K, μeff 8.1 μB for x= 0.12, θCW= 18.14(7) K, μeff 8.2 μBfor x= 0.2, and θCW= 29.35(9) K, μeff 8.3 μB for x= 1. The ob-tained values of μeff are close to the theoretical value of a free Eu2+ion (μEu2+= 7.94 μB).
As shown in Fig.2, for all the P substituted samples an obvious deviation between χZFCand χFCis seen at low tem-peratures. This is not the case for x= 0 [18,21], for which AFM order of Eu2+ with the moments pointing along the a axis was reported. This result is consistent with previous magnetizaton studies , suggesting that the ground state of the coupled Eu2+spins is a canted AFM state (C-AFM state) (i.e., AFM with the net ferromagnetic (FM) compo-nent along the c-axis) in EuFe2(As1−xPx)2(x= 0.12, 0.2) and a FM state in EuFe2P2. Recently, neutron diffraction measurements were also performed on EuFe2P2and an al-most axial FM structure of the Eu2+spins was established . The C-AFM and FM structure of the Eu-sublattice in EuFe2(As1−xPx)2(x= 0.12, 0.2, 1) sharply contrasts with the planar antiferromagnetism seen in the parent compound EuFe2As2, suggesting a delicate interplay between the Eu 4f and the Fe 3d electrons. It was concluded from different experiments [12,13] that there is a strong coupling between the localized Eu2+spins and the conduction electrons of the two-dimensional (2D) Fe2As2layers in EuFe2As2. This re-vealed that the magnetic exchange interaction between the
Fig. 3 ZF μSR spectra for
EuFe2(As1−xPx)2(x= 0, 0.12,
0.2, 1) recorded for three different temperatures: T < TEu
(circles), TEu< T < TSDW
(diamonds), and T > TSDW
(spheres). The solid lines represent fits to the data by means of Eq. (2)
localized Eu 4f moments is mediated by the itinerant Fe 3d electrons. However, the interaction of the Eu moments with the magnetic moments of the Fe sublattice (band mag-netism) cannot be neglected. Only a combination of both interactions can further elucidate the C-AFM ground state observed in EuFe2(As1−xPx)2(x= 0.12 and 0.2). Note that a C-AFM ground state was also found in the related com-pound EuFe1.8Co0.2As2.
The magnetic ordering temperature TEuof the Eu2+ mo-ments was determined by the temperature at which the dif-ference between χZFC and χFC sets in (see the inset of Fig. 2). It was found to be TEu 16.5, 18, and 29 K for x= 0.12, x = 0.2, and x = 1, respectively. The value of TEu for x= 0.12 is slightly reduced compared to TEu 19 K for the parent compound x= 0. However, on further increasing the P concentration TEuincreases and reaches a maximum for x= 1. The value of TEufor x= 1 is in agreement with those reported in literature [19,25,27].
3.1.3 Zero-Field μSR Measurements
In a μSR experiment, nearly 100 % spin-polarized muons μ+are implanted into the sample one at a time. The pos-itively charged μ+ thermalize at interstitial lattice sites, where they act as magnetic microprobes. In a magnetic material, the muon spin precesses in the local magnetic field Bμ at the muon site with the Larmor frequency νμ = γμ/(2π )Bμ (muon gyromagnetic ratio γμ/(2π )= 135.5 MHz T−1). ZF μSR is a very powerful tool to in-vestigate microscopic magnetic properties of solids without applying an external magnetic field.
ZF μSR time spectra for the single crystal of EuFe2As2 and for the polycrystalline samples EuFe2(As1−xPx)2 are shown in Fig.3, recorded for three different temperatures: T < TEu, TEu< T < TSDW, and T > TSDW. For EuFe2As2, the ZF μSR measurements were performed with the initial muon spin polarization tilted by approximately 45◦ away from the crystallographic c-axis. At high temperatures (see Fig.3), no muon spin precession and only a very weak polarization of the μSR signal is observed. This weak de-polarization and its Gaussian functional form are typical for a paramagnetic material and reflect the occurrence of a small Gaussian–Kubo–Toyabe depolarization, originating from the interaction of the muon spin with randomly ori-ented nuclear magnetic moments. At temperatures below TEua well-defined spontaneous muon spin precession is ob-served in all compounds, indicating long-range magnetic or-der of the Eu2+ moments in the investigated compounds. For x= 0 and 0.12 above TEu 20.5 and 16.5 K, respec-tively, muon spin precession with a lower frequency is ob-served which is caused by the long-range SDW order of the Fe moments. However, for x= 0.2, instead of the oscilla-tory behavior seen in the SDW state for x= 0 and 0.12, a fast decaying signal is observed (see Fig.3(c)). The rea-son for this strongly decaying μSR signal will be discussed below. For x= 1, only the magnetic ordering of the Eu mo-ments is seen in the μSR spectra (Fig.3(d)). Note that for x= 0, 0.12 and 0.2 only one μSR frequency is visible. How-ever, for x= 1 two distinct precession frequencies occur in the μSR spectra, corresponding to the local magnetic fields Bμ,Eu1 1.08 T (70 % of the signal) and Bμ,Eu2 1.37 T
Fig. 4 The temperature dependence of the internal magnetic field Bi μ
for the samples EuFe2(As1−xPx)2(x= 0, 0.12, 0.2, and 1). The solid
lines represent fits to the data by means of Eq. (3). The arrows mark the transition temperatures for the SDW (TSDW) and the Eu magnetic
(30 % of the signal). This indicates that two magnetically inequivalent muon stopping sites are present in EuFe2P2.
The ZF μSR data were analyzed using the following functional form: A(t )= 2 i=1 Ai0αie−λ i TtcosγμBi μt+ ϕ + βie−λ i Lt. (2)
αi and βi= 1 − αi (i= 1 for x = 0, 0.12, 0.2, and i = 1, 2 for x= 1) are the fractions of the oscillating and nonoscil-lating μSR signal. For the single crystal (x= 0) one finds α1= 0.73(2) and β1= 0.27(3). However, for the polycrys-talline samples αi= 2/3 and βi = 1/3. The 2/3 oscillating and the 1/3 nonoscillating μSR signal fractions originate from the spatial averaging in powder samples where only 2/3 of the magnetic field components are perpendicular to the muon spin and cause muon spin precession. A0denotes the initial asymmetry, and ϕ is the initial phase of the muon-spin ensemble. Bi
μrepresents the internal magnetic field at the muon site, and the depolarization rates λiT and λiL char-acterize the damping of the oscillating and nonoscillating part of the μSR signal, respectively. The transversal relax-ation rate λiT is a measure of the width of the static mag-netic field distribution at the muon site, and also reflects dynamical effects (spin fluctuations). The longitudinal re-laxation rate λiL is determined by dynamic magnetic fluc-tuations only . The temperature dependence of the in-ternal magnetic field Bi
μ for EuFe2(As1−xPx)2is shown in Fig.4. Bi
μ is proportional to the magnitude of the ordered moment and thus to the magnetic order parameter. The sec-ond component (i= 2) in the μSR signal was observed only for x= 1, and hence, we will discuss the x-dependence of
the relevant physical parameters related to the first compo-nent (i= 1) only. For x = 0 a sharp step like increase of Bμ1 is observed below195 K, which reflects the appearance of the SDW ordering of the Fe moments. The value of TSDWis in good agreement with TSDW 190 K obtained from neu-tron diffraction . A sharp increase of Bμ1 is an indica-tion for a first order transiindica-tion. A first order transiindica-tion due to SDW formation was also observed in the related com-pound SrFe2As2 . Upon lowering the temperature Bμ1 first tends to saturate, but increases again when the mag-netic order of the Eu2+moments occurs at TEu. To describe the temperature dependence of Bμi, we assumed the follow-ing phenomenological function:
Bμi(T )= Bμ,Eui (0) 1− T TEu γ1δ1 + Bμ,SDWi (0) 1− T TSDW γ2δ2 , (3)
where Bμ,Eui (0) and Bμ,SDWi (0) represent the zero-temper-ature values of the internal magnetic field probed by the muons in the Eu and in the SDW ordered states, respectively. γ and δ are empirical exponents. As indicated by the solid lines in Fig.4the function in Eq. (3) describes the data rea-sonably well, yielding the parameters given in Table1. Note that with increasing x the values of TSDWand Bμ,SDW1 (0) de-crease, and for x= 0.2 and x = 1 no long-range SDW order of the Fe moments is observed. On the other hand, TEu de-creases with increasing x, reaches minimum at x= 0.12 and then increases again, in agreement with the above suscepti-bility measurements. In addition, Bμ,Eu1 (0) significantly in-creases with x above x= 0.12. Considering the magnetiza-tion results, the increase of Bμ,Eu1 (0) may be ascribed to the appearance/growth of the ferromagnetic component as a re-sult of P substitution. However, without microscopic mod-eling (i.e., calculation of the μ stopping site and the dipo-lar fields at the μ site) it is not possible to conclude how a change of the magnetic structure with P substitution would affect the internal field at the muon site.
The temperature dependences of the transverse and lon-gitudinal depolarization rates λ1T and λ1L are presented in Fig.5(a) and (b), respectively. Note that λ1T is much smaller for the end members x= 0, 1 of the investigated system than for the mixed compounds x= 0.12, 0.2. As shown in Fig. 5(a), for x = 0, 0.12, and 0.2, the onset of the Fe magnetic order is accompanied by an increase of λ1T that decreases with decreasing temperature. Upon reaching the magnetic ordering temperature of Eu λ1T shows another maximum. For x= 1, the strong increase of λ1T around TEu is only due the Eu order. No SDW transition is observed at higher temperatures. The magnetic ordering temperatures of Eu (TEu) and Fe (TSDW) are also clearly visible in the longi-tudinal relaxation rate λ1L, which also shows a clear anomaly
Table 1 Summary of the parameters obtained for the polycrystalline
samples of EuFe2(As1−xPx)2(x= 0, 0.12, 0.2, 1) by means of
mag-netization and μSR experiments. TEuχ and TEuμSR are the magnetic ordering temperatures of the Eu moments determined by susceptibility and μSR measurements. TSDWdenotes the SDW ordering temperature
of the Fe moments determined from μSR experiments. Bi
μ,SDW(0) (i= 1, 2) represent the zero-temperature values of the
in-ternal magnetic fields at the muon site probed in the Eu and the SDW ordered state x TEuχ (K) TEuμSR(K) TSDW(K) Bμ,Eu1 (0) (T) Bμ,Eu2 (0) (T) Bμ,SDW1 (0) (T) Bμ,SDW2 (0) (T) 0 19.5(6) 20.5(5) 195(3) 0.45(1) – 0.35(1) – 0.12 16.5(5) 16.7(6) 140(5) 0.476(12) – 0.258(10) – 0.2 17.9(5) 18.4(2) 85 0.997(12) – 0 – 1 29.5(5) 29.3(4) 0 1.08(1) 1.37(2) 0 0
Fig. 5 (a) Transverse relaxation rate λ1T (T) for the samples EuFe2(As1−xPx)2with x= 0, 0.12, 0.2, and 1. Lines are guides to
the eye. (b) Longitudinal relaxation rate λ1L(T) for EuFe2(As1−xPx)2
(x= 0, 0.12, 0.2, 1). The arrows mark the transition temperatures for the high-temperature SDW (TSDW) and the low-temperature Eu order
at TEuand TSDW(see Fig.5(b)). As mentioned above, for the sample with x= 0.2 (see Fig.3(c), diamonds) only a fast de-polarization of the implanted muons is observed above TEu, but no coherent precession signal. The fast depolarization of the μSR signal could be either due to a wide distribution of static fields, and/or to strongly fluctuating magnetic mo-ments. To discriminate between these two possibilities we compare the values of λ1T and λ1L. Note that for x= 0.2, and T < 85 K λ1T is very large (50 MHz) while λ1L is small (0.05 MHz). λ1
T consists of a static as well as of a dynamic contribution, while λ1Lcontains only a dynamic contribution. Since in our case λ1T λ1L, the static contribu-tion dominates λ1T, and the fast depolarization of the μSR signal observed for x= 0.2 is due to the (quasi-)static dis-ordered SDW phase with TSDW 85 K. The important pa-rameters for all samples extracted from the magnetization and the μSR experiments are summarized in Table1.
Very recently, bulk superconductivity with Tc 28 K was reported in single crystals of P substituted EuFe2(As1−xPx)2  based on resistivity, magnetization, and specific heat measurements. However, superconductiv-ity coexisting with AFM Eu2+ order was only found in a very narrow x range (0.16≤ x ≤ 0.22), where the SDW transition is suppressed. In the present study, no indication of superconductivity was seen for x= 0.2 from magneti-zation measurements. This might be due to the fact that in our sample (x= 0.2) the SDW state is not completely sup-pressed as supported by the μSR measurements. In addition to chemical pressure, the physical properties of EuFe2As2 can be also tuned by the application of hydrostatic pressure [6,20]. Previous reports of high pressure experiments on EuFe2As2revealed pressure-induced superconductivity in a narrow pressure range of 2.5–3.0 GPa [6,20], accompanied by a suppression of the SDW state of the Fe moments. Since pressure experiments on EuFe2As2 were already reported by various groups [6,20], we decided to study pressure ef-fects in the P substituted sample EuFe2(As0.88P0.12)2. The sample with x = 0.12 was chosen for the following rea-sons: (i) According to the SC phase diagram reported  for EuFe2As2 as a function of chemical pressure (P
con-tent x), the sample with x= 0.12 is close to the value of x at which superconductivity appears. By applying hydro-static pressure, the SC phase might be reachable. (ii) Based on previous reports [6,20], superconductivity was found in the vicinity of the pressure value where the SDW state is suppressed.
In the following sections, the results of the magnetization and the μSR experiments performed on EuFe2(As0.88P0.12)2 under hydrostatic pressures are presented.
3.2 Hydrostatic Pressure Effect on EuFe2(As0.88P0.12)2 3.2.1 High Pressure Magnetization Measurements
Magnetization measurements were carried out under hydro-static pressures up to p = 5.9 GPa. The temperature de-pendence of the ZFC and FC magnetic susceptibilities χ for EuFe2(As0.88P0.12)2 recorded at ambient and selected applied pressures is shown in Fig. 6(a) (p≤ 0.4 GPa), in Fig. 6(b) (0.42 GPa≤ p ≤ 0.55 GPa), and in Fig. 6(c) (1.1 GPa≤ p ≤ 5.9 GPa). Note that Fig.6shows the data after subtraction of the background signal from the empty pressure cell. The magnetic ordering temperature TEuof the Eu2+moments was determined as described in Sect.3.1.2. At ambient pressure, a clear bifurcation between the ZFC and FC curves appears below TEu 16.5 K, which is con-sistent with the susceptibility data obtained for the sample without pressure cell (see Fig. 2). In addition, the mag-nitudes of the susceptibilities are also in fair agreement. Upon increasing the pressure, an anomaly in the ZFC sus-ceptibility is observed at p= 0.4, 0.42, and 0.48 GPa as shown in Fig. 6(a) and (b). The low-temperature data for p = 0.4 GPa are shown in the inset of Fig. 6(a). In ad-dition to the Eu order observed at 18 K, a strong de-crease of the ZFC susceptibility is observed at 11 K, which is possibly due to the appearance of superconductiv-ity. The decrease of the susceptibility corresponds to nearly 100 % diamagnetic shielding. In order to confirm supercon-ductivity, transport measurements under pressure are nec-essary. Just magnetization data do not allow to conclude that the observed decrease of χZFC is due to the appear-ance of superconductivity. Hence we call this phase “X”. For p = 0.42 GPa, the susceptibility also shows a pro-nounced decrease at TX 20 K (see Fig. 2(b), the low-temperature data are shown in the inset). Below 18.2 K, the susceptibility starts to increase again due to the C-AFM ordering of the Eu2+ moments. Upon increasing the pres-sure to p= 0.47 GPa, the transition temperature TX de-creases to 8.8 K. Above p = 0.55 GPa, the “X” phase is no longer visible (see Fig. 6(c)). It is also absent for p <0.35 GPa. Therefore, pressure-induced “X” phase in EuFe2(As0.88P0.12)2 is very likely present in a very nar-row pressure range. We observed that TEu increases upon
Fig. 6 Temperature dependence of the ZFC and FC magnetic
suscep-tibility of EuFe2(As0.88P0.12)2 in a magnetic field of μ0H= 2 mT
for p≤ 0.4 GPa (a), for 0.42 GPa ≤ p ≤ 0.55 GPa (b), and for 1.1 GPa≤ p ≤ 5.9 GPa (c). The arrows mark the ordering tempera-ture of Eu moments (TEu) and the “X” transition temperatures (TX).
The insets of panels (a) and (b) show the low temperature data for
p= 0.4 GPa and 0.42 GPa, respectively, illustrating the transition to
the superconducting state marked by the arrows. The solid lines are guides to the eye
increasing hydrostatic pressure, similar to chemical pres-sure. The maximum value of TEu = 56 K is reached at p= 5.6 GPa, and at higher pressures it tends to decrease (see Fig.6(c)). For instance, TEu= 53 K at the maximum applied pressure p= 5.9 GPa. A maximum of TEuwas also
Fig. 7 ZF μSR spectra of
at p= 0.0, 0.66, 1.1, and 2 GPa, recorded for three different temperatures: T < TEu(circles),
TEu< T < TSDW(diamonds),
and T > TSDW(spheres). The
solid lines represent fits to the
data by means of Eq. (4)
observed for the parent compound EuFe2As2, but at higher pressure (p= 8 GPa). According to recent X-ray diffrac-tion studies  of EuFe2As2, a collapsed tetragonal (cT) phase was found above 8 GPa. It is known that the pressure-induced structural transition toward the cT phase is con-nected with a valence change of the Eu ions, as reported for EuFe2P2and EuCo2P2. Therefore, it is possible that the decrease of TEuabove 5.6 GPa is connected with a pressure-induced valence change from the magnetic Eu2+to the non-magnetic Eu3+ state. However, to gain further insight into this pressure region, measurements at p > 5.9 GPa are nec-essary.
3.2.2 Zero-Field μSR Measurements Under Pressure Hydrostatic pressure effects on the magnetic properties of EuFe2(As0.88P0.12)2 were studied microscopically by means of ZF μSR. Some representative μSR time spectra at different applied pressures are shown in Fig.7. A substan-tial fraction of the μSR asymmetry signal originates from muons stopping in the MP35N pressure cell  surround-ing the sample. Therefore, the total μSR asymmetry is a sum of two components:
AZF(t )= AZFS (t )+ AZFPC(t ), (4) AZFS (t )is the contribution of the sample, and AZFPC(t )is the contribution of the pressure cell. AZFS (t ) is well described
by Eq. (2) with α1= 2/3 and β1= 1/3 (since for x = 0.12 the μSR spectra contain only one frequency, α2= 0 and β2= 0). The signal of the pressure cell was analyzed by a damped Kubo–Toyabe (KT) function :
AZFPC(t )= AZFPC(0) 1 3+ 2 3(1− σ t)e −σ2t2/2 e−λt. (5)
Here AZFPC(0) is the amplitude of AZFPC(t )at t= 0. The width of the static Gaussian field distribution σ = 0.338 µ s−1 and the damping rate λ= 0.04 µ s−1 were obtained from a measurement of the empty pressure cell. The total ini-tial asymmetry is AZFS (0) + AZFPC(0) = 0.29. The ratio AZFS (0)/[AZFS (0)+ AZFPC(0)] 40 % implies that approxi-mately 40 % of the muons are stopping in the sample. Up to p= 1.1 GPa the spontaneous muon-spin precession in the Eu ordered and in the SDW state is clearly observed in the ZF μSR time spectra (see Fig. 7), indicating long range magnetic order in the Eu and the Fe sublattice. Above p= 1.1 GPa the SDW state is suppressed and only the magnetic order of the Eu moments remains. The tempera-ture dependence of the internal field Bμ1 for various hydro-static pressures is shown in Fig.8. The inset shows Bμ,Eu1 at low temperatures where the magnetic ordering of the Eu2+ moments is evident. The data were analyzed by Eq. (3). The SDW ordering temperature TSDW of the Fe moments (TSDW= 140 K at ambient pressure) as well as Bμ,SDW1 created by the Fe sublattice decrease with increasing pres-sure. Above p= 1.1 GPa, the SDW order is completely suppressed. On the contrary, TEu increases with pressure,
in agreement with the susceptibility measurements. In addi-tion, Bμ,Eu1 related to the Eu ordered state also increases with pressure. Note the sharp increase of Bμ,Eu1 below TEuwith increasing the pressure from p= 0 GPa to p = 0.44 GPa. For p > 0.44 GPa, a more smooth increase of Bμ,Eu1 is observed. Relevant parameters of EuFe2(As0.88P0.12)2 tracted from the high pressure magnetization and μSR ex-periments are listed in Table2.
As shown above the magnetization measurements indi-cate the presence of a possible SC phase in the pressure
Fig. 8 Temperature dependence of the internal field B1
μat the muon
site for the sample EuFe2(As0.88P0.12)2 recorded at various applied
pressures. The solid lines represent fits to the data by means of Eq. (3).
The arrows mark the ordering temperature TSDW. The inset shows the
low temperature data, illustrating the transition at TEuto the
magneti-cally ordered state of the Eu moments
range 0.36 GPa≤ p ≤ 0.5 GPa. An attempt to detect it in the sample EuFe2(As0.88P0.12)2with ZF and TF μSR, failed be-cause of the strong intrinsic magnetism present in the sam-ple.
4 Phase Diagram
Figure9(a) shows the (x–T ) phase diagram for the system EuFe2(As1−xPx)2. The (p–T ) phase diagram of EuFe2(As0.88P0.12)2is plotted in Fig.9(b). The data for TEu represented by the triangles in Fig.9(a) are taken from . In the (x–T ) phase diagram, three different phases were identified: a paramagnetic phase (PM), spin-density wave order of the Fe moments (SDW), and magnetic order of Eu2+ moments (MO). Moreover, in the (p–T ) phase dia-gram, pressure-induced “X” phase was found (see the inset of Fig.9(b)). In Fig.10, the internal magnetic fields Bμ,Eu1 and Bμ,SDW1 probed by the muons in the Eu ordered and in the SDW state and the low temperature value of the mag-netic susceptibility χZFC(7 K) are plotted as a function of P content x and applied pressure p.
By combining the above phase diagrams, one obtains a coherent physical picture on the system EuFe2As2 upon P substitution and on EuFe2(As0.88P0.12)2 under hydro-static pressure. An important finding is the observation of pressure-induced “X” phase in EuFe2(As0.88P0.12)2, coex-isting with magnetic order of the Eu and Fe moments. “X” phase appears in the narrow pressure region of 0.36– 0.5 GPa. The presented phase diagrams in combination with the results obtained for the parent compound under pres-sure [6,20] allow us to draw the following conclusion on
Table 2 Summary of the
parameters obtained for the polycrystalline sample of EuFe2(As0.88P0.12)2at different
hydrostatic pressures by means of magnetization and μSR experiments. The meaning of the symbols is given in the text
p(GPa) TEuχ (K) TEuμSR(K) TX(K) TSDWμSR(K) Bμ,Eu1 (0) (T) Bμ,SDW1 (0) (T) 0 16.5(5) 16.4(3) – 141.2(1) 0.44(1) 0.25(1) 0.4 17.5(4) – 11.2(3) – – – 0.42 17.6(5) – 20.3(3) – – – 0.44 – 17.7(3) - 110(1) 0.99(2) 0.19(2) 0.48 17.9(4) – 7.3(3) – – – 0.66 18.9(5) 18.4(6) 0 75(2) 1.07(5) 0.17(4) 1.1 20.5(5) 19.9(7) 0 40(3) 1.27(3) 0.12(2) 1.73 24.6(3) – 0 – – – 1.97 24.4(5) 23.6(7) 0 0 1.23(2) 0 2.5 27.2(3) – 0 – – – 3.85 35.8(5) – 0 – – – 4.54 42.5(4) – 0 – – – 5.1 49.5(3) – 0 – – – 5.6 57(4) – 0 – – – 5.9 53(5) – 0 – – –
Fig. 9 (a) (x–T ) phase diagram of EuFe2(As1−xPx)2. The data points
represented by the triangles are taken from . (b) (p–T ) phase di-agram of EuFe2(As0.88P0.12)2. The various phases in the phase
dia-grams and the corresponding transition temperatures are denoted as follows: paramagnetic (PM), spin-density wave (SDW) and TSDW,
magnetic ordering of Eu (MO) and TEu, “X” phase (the meaning of this
phase is given in the text) and TX. For clarity, the inset in (b) shows the
“X” phase present in a very narrow pressure range
the relation between chemical and hydrostatic pressure in EuFe2As2:
1. Both chemical and hydrostatic pressure suppress TSDW and Bμ,SDW1 (0). However, the SDW ground state is dif-ferently affected by x and p. At all applied pressures be-low p= 1.1 GPa long-range SDW order was observed, while in the case of chemical pressure for x= 0.2 a dis-ordered SDW phase exist. This may be related to the fact that by chemical pressure (P substitution) considerably more disorder is introduced.
2. Figure 9 shows that in the case of P substitution TEu first decreases as a function of x, reaches a minimum at x= 0.12, and then increases. For a fixed P content of x= 0.12, the ordering temperature TEuincreases with pressures up to p= 5.6 GPa. Above p = 5.6 GPa,
how-Fig. 10 Zero-temperature values of the internal magnetic fields B1 μ,Eu
and Bμ,SDW1 and the low-temperature value of the magnetic suscepti-bility χZFCas a function of the P content x (a) and applied pressure (b)
ever, TEu(p)decreases, accompanied by a possible va-lence change of the Eu moments. In the parent compound EuFe2As2, a valence change was found at a higher pres-sure p= 8 GPa.
3. The internal magnetic field Bμ,Eu1 (0) in the Eu ordered state increases with increasing x as well as by applying hydrostatic pressure (see Fig.10(a)–(b)).
4. The low temperature value of the magnetic susceptibility χZFC (7 K) first increases with increasing x and p and above some critical values (x= 0.2 and p = 1.1 GPa) it decreases (see Fig.10(a)–(b)).
By considering the findings listed above, the qualitative statement can be made that the properties of EuFe2(As1−xPx)2 are similarly tuned by chemical and hy-drostatic pressure.
In summary, the magnetic and superconducting properties of the system EuFe2(As1−xPx)2(x= 0, 0.12, 0.2, 1) were studied by magnetization and μSR experiments. In addition, the sample with x= 0.12 was also investigated by applying hydrostatic pressure up to p 5.9 GPa. The (x–T ) phase di-agram of EuFe2(As1−xPx)2and the (p–T ) phase diagram of
EuFe2(As0.88P0.12)2were determined and discussed as well as compared to the (p–T ) phase diagram recently obtained for EuFe2As2[6,20]. The present investigations reveal that the magnetic coupling between the Eu and the Fe sublat-tices strongly depends on chemical and hydrostatic pressure and determines the (x–T ) and (p–T ) phase diagrams as pre-sented in this work. According to the above discussed phase diagrams, chemical and hydrostatic pressures have qualita-tively a similar effect on the Fe and Eu magnetic order.
There are still some open questions related to supercon-ductivity and its interplay with the magnetic ground state of the system EuFe2As2. One of the most interesting aspects of this particular member of Fe-based superconductors is the possibility to observe coexistence or competition between superconductivity and rare-earth Eu magnetic order. In the present work, the so-called “X” phase induced by pressure was observed in EuFe2(As0.88P0.12)2in addition to the mag-netic phases of the Eu and Fe sublattices. It exists in a narrow pressure range 0.36–0.5 GPa. This phase is possibly super-conducting. However, transport measurements as a function of pressure are required in order to clarify this point.
Acknowledgements This work was supported by the Swiss Na-tional Science Foundation, the SCOPES grant No. IZ73Z0_128242, and the NCCR Project MaNEP. The μSR experiments were performed at the Swiss Muon Source of the Paul Scherrer Institute (PSI), Villigen, Switzerland.
1. Kamihara, Y., Watanabe, T., Hirano, M., Hosono, H.: J. Am. Chem. Soc. 130, 3296 (2008)
2. Rotter, M., Tegel, M., Johrendt, D.: Phys. Rev. Lett. 101, 107006 (2008)
3. Chen, X.H., Wu, T., Wu, G., Liu, R.H., Chen, H., Fang, D.F.: Na-ture (London) 453, 761 (2008)
4. Torikachvili, M.S., Bud’ko, S.L., Ni, N., Canfield, P.C.: Phys. Rev. Lett. 101, 057006 (2008)
5. Fukazawa, H., Takeshita, N., Yamazaki, T., Kondo, K., Hirayama, K., Kohori, Y., Miyazawa, K., Kito, H., Eisaki, H., Iyo, A.: J. Phys. Soc. Jpn. 77, 105004 (2008)
6. Terashima, T., Kimata, M., Satsukawa, H., Harada, A., Hazama, K., Uji, S., Suzuki, H.S., Matsumoto, T., Murata, K.: J. Phys. Soc. Jpn. 78, 083701 (2009)
7. Ren, Z.A., Lu, W., Yang, J., Yi, W., Shen, X.L., Li, Z.C., Che, G.C., Dong, X.L., Sun, L.L., Zhou, F., Zhao, Z.X.: Chin. Phys. Lett. 25, 2215 (2008)
8. Matsuishi, S., Inoue, Y., Nomura, T., Hirano, M., Hosono, H.: J. Phys. Soc. Jpn. 77, 113709 (2008)
9. Zhao, J., Huang, Q., de la Cruz, C., Li, S., Lynn, J.W., Chen, Y., Green, M.A., Chen, G.F., Li, G., Li, Z., Luo, J.L., Wang, N.L., Dai, P.: Nat. Mater. 7, 953 (2008)
10. Raffius, H., Mörsen, M., Mosel, B.D., Müller-Warmuth, W., Jeitschko, W., Terbüchte, L., Vomhof, T.: J. Phys. Chem. Solids
54, 135 (1993)
11. Xiao, Y., Su, Y., Meven, M., Mittal, R., Kumar, C.M.N., Chatterji, T., Price, S., Persson, J., Kumar, N., Dhar, S.K., Thamizhavel, A., Brueckel, T.: Phys. Rev. B 80, 174424 (2009)
12. Jiang, S., Luo, Y.K., Ren, Z., Zhu, Z.W., Wang, C., Xu, X.F., Tao, Q., Cao, G.H., Xu, Z.A.: New J. Phys. 11, 025007 (2009) 13. Guguchia, Z., Roos, J., Shengelaya, A., Katrych, S., Bukowski, Z.,
Weyeneth, S., Murányi, F., Strässle, S., Maisuradze, A., Karpinski, J., Keller, H.: Phys. Rev. B 83, 144516 (2011)
14. Sefat, A.S., Jin, R., McGuire, M.A., Sales, B.C., Singh, D.J., Man-drus, D.: Phys. Rev. Lett. 101, 117004 (2008)
15. Leithe-Jasper, A., Schnelle, W., Geibel, C., Rosner, H.: Phys. Rev. Lett. 101, 207004 (2008)
16. He, Y., Wu, T., Wu, G., Zheng, Q.J., Liu, Y.Z., Chen, H., Ying, J.J., Liu, R.H., Wang, X.F., Xie, Y.L., Yan, Y.J., Dong, J.K., Li, S.Y., Chen, X.H.: J. Phys. Condens. Matter 22, 235701 (2010) 17. Li, L.J., Luo, Y.K., Wang, Q.B., Chen, H., Ren, Z., Tao, Q., Li,
Y.K., Lin, X., He, M., Zhu, Z.W., Cao, G.H., Xu, Z.A.: New J. Phys. 11, 025008 (2008)
18. Ren, Z.: Phys. Rev. B 79, 094426 (2009)
19. Jeevan, H.S., Kasinathan, D., Rosner, H., Gegenwart, P.: Phys. Rev. B 83, 054511 (2011)
20. Matsubayashi, K., Munakata, K., Isobe, M., Katayama, N., Oh-gushi, K., Ueda, Y., Uwatoko, Y., Kawamura, N., Mizumaki, M., Ishimatsu, N., Hedo, M., Umehara, I.: Phys. Rev. B 84, 024502 (2011)
21. Guguchia, Z., Bosma, S., Weyeneth, S., Shengelaya, A., Puz-niak, R., Bukowski, Z., Karpinski, J., Keller, H.: Phys. Rev. B 84, 144506 (2011)
22. Rodrígues-Carvajal, J.: Physica B 192, 55 (1993) 23. Andreica, D.: Ph.D. Thesis, IPP/ETH-Zürich (2001) 24. Suter, A., Wojek, B.M.: Phys. Procedia 30, 69–73 (2012) 25. Cao, G., Xu, S., Ren, Z., Jiang, S., Feng, C., Xu, Z.: J. Phys.
Con-dens. Matter 23, 464204 (2011) (5 pp.)
26. Zapf, S., Wu, D., Bogani, L., Jeevan, H.S., Gegenwart, P., Dressel, M.: Phys. Rev. B 84, 140503(R) (2011)
27. Ryan, D.H., Cadogan, J.M., Xu, S., Xu, Z., Cao, G.: Phys. Rev. B
83, 132403 (2011)
28. Maeter, H., Luetkens, H., Pashkevich, Yu.G., Kwadrin, A., Khasanov, R., Amato, A., Gusev, A.A., Lamonova, K.V., Chervin-skii, D.A., Klingeler, R., Hess, C., Behr, G., Büchner, B., Klauss, H.H.: Phys. Rev. B 80, 094524 (2009)
29. Jesche, A., Caroca-Canales, N., Rosner, H., Borrmann, H., Ormeci, A., Kasinathan, D., Klauss, H.H., Luetkens, H., Khasanov, R., Amato, A., Hoser, A., Kaneko, K., Krellner, C., Geibel, C.: Phys. Rev. B 78, 180504(R) (2008)
30. Uhoya, W., Tsoi, G., Vohra, Y.K., McGuire, M.A., Sefat, A.S., Sales, B.C., Mandrus, D., Weir, S.T.: J. Phys. Condens. Matter 22, 292202 (2010)
31. Ni, B., Abd-Elmeguid, M.M., Micklitz, H., Sanchez, J.P., Vulliet, P., Johrendt, D.: Phys. Rev. B 63, 100102 (2001)